photostimuli with the linkers serving as photon antennae. Theoretical calculations show that MOFs are semiconductors or insulators with band gaps between 1.0 and 5.5 eV which can be altered by changing the degree of conjugation in the ligands. Experimental results show that the band gap of IRMOF-type samples can be tuned by varying the functionality of the linker. An integrated MOF nanozyme was developed for anti-inflammation therapy. Mechanical Properties Implementing MOFs in industry necessitates a thorough understanding of the mechanical properties since most processing techniques (e.g. extrusion and pelletization) expose the MOFs to substantial mechanical compressive stresses. The mechanical response of porous structures is of interest as these structures can exhibit unusual response to high pressures. While zeolites (microporous, aluminosilicate minerals) can give some insights into the mechanical response of MOFs, the presence of organic linkers as opposed to zeolites, makes for novel mechanical responses. MOFs are very structurally diverse meaning that it is challenging to classify all of their mechanical properties. Additionally, variability in MOFs from batch to batch and extreme experimental conditions (Diamond anvil cells) mean that experimental determination of mechanical response to loading is limited, however many computational models have been made to determine structure-property relationships. Main MOF systems that have been explored are zeolitic imidazolate frameworks (ZIFs), Carboxylate MOFs, Zirconium-based MOFs, among others. Generally, the MOFs undergo three processes under compressive loading (which is relevant in a processing context): amorphization, hyperfilling, and/or pressure induced phase transitions. During amorphization linkers buckle and the internal porosity within the MOF collapses. During hyperfilling the MOF which is being hydrostatically compressed in a liquid (typically solvent) will expand rather than contract due to a filling of pores with the loading media. Finally, pressure induced phase transitions where the structure of the crystal is altered during the loading are possible. The response of the MOF is predominantly dependent on the linker species and the inorganic nodes. Zeolitic Imidazolate Frameworks (ZIFs) Several different mechanical phenomena have been observed in zeolitic imidazolate frameworks (ZIFs), the most widely studied MOF for mechanical properties due to their many similarities to zeolites. General trends for the ZIF family are the tendency of the Young's modulus and hardness of the ZIFs to decrease as the accessible pore volume increases. The bulk moduli of ZIF-62 series increase with the increasing of benzoimidazolate (bim−) concentration. ZIF-62 shows a continuous phase transition from open pore (op) to close pore (cp)